Template-Assisted Sol-Gel Synthesis of Nanocrystalline BaTiO · PDF fileθ, degrees...
Embed Size (px)
Transcript of Template-Assisted Sol-Gel Synthesis of Nanocrystalline BaTiO · PDF fileθ, degrees...
ISSN: 0973-4945; CODEN ECJHAO
E-Journal of Chemistry
http://www.e-journals.net 2010, 7(3), 894-898
Template-Assisted Sol-Gel Synthesis of
Department of Materials Engineering,
Indian Institute of Science, Bangalore 560 012, India.
Received 28 October 2009; Accepted 20 December 2009
Abstract: Nanocrystalline perovskite barium titanate with an average particle
size less than ~10 nm is produced using sol-gel route involving ligand-assisted
templating. BaTiO3 is obtained by the controlled hydrolysis and condensation
reaction of barium acetate (Ba(CH3COO)2) with titanium tetra chloride (TiCl4)
in the reverse micelles of dodecylamine (DDA) which is used as the template.
Our attempts to produce mesoporous BaTiO3 have resulted in the formation of
nanocrystalline BaTiO3. The synthesis of nanostructured BaTiO3 is carried out
using the ligand-assisted templating approach which proceeds through the
sol-gel route. Dodecylamine is used as the template. The sol-gel process in
general presents inherent advantages because the nanostructure of the desired
materials can be controlled together with their porous structure. Ligand-assisted
templating approach involves the formation of covalent bond between the
inorganic analogue and the template. Ba(CH3COO)2 and TiCl4 are used as
barium-source and titanium-source respectively. The reaction between
Ba(CH3COO)2 and TiCl4 is found to take place deliberately on the pre-
assembled species which acts as the template or occurring with in them which
in turn will lead to the generation of the desired nanoscale structure (nanopores
Keywords: Ligand-assisted templating; Ba(CH3COO)2, TiCl4, Dodecylamine; XRD, TEM.
Barium titanate (BaTiO3) is well-known for its high dielectric constant. The dielectric
properties are controlled by purity and microstructure which in turn are dependent on the
method of preparation1. Recent advances in nanotechnology such as: Multilayer capacitor,
Micro Electro Mechanical Systems and Dynamic Random Access Memories have resulted
in the miniaturization of devices2. These require nanosize BaTiO3. Various chemical routes
like coprecipitation3, sol-gel
5-6 and solution combustion
7 are known to yield
Template-Assisted Sol-Gel Synthesis of Nanocrystalline BaTiO3 895
nanoparticle products. Applying meso-scale design strategies to perovskite compounds is a
very interesting topic and may bring new exciting discoveries in these widely utilized
materials, especially when considering the current and future needs for functionalized
materials to perform smart functions. The synthesis of mesoporous BaTiO3 by template-
assisted sol-gel process is earlier reported where tetradecylamine is used as template8. There
is also a report on the synthesis of mesoporous BaTiO3 using cationic surfactants like
cetyltrimethyl ammonium chloride9 as template. But the synthesis of mesoporous BaTiO3
using dodecylamine as the template is attempted here which indeed resulted in the formation
of nanocrystalline BaTiO3. The synthesis of nanocrystalline BaTiO3 through templating
approach is first of its kind.
To 1 g of dodecylamine (DDA) in 5 mL of isopropanol, 1 mL of TiCl4 in 2 mL of
isopropanol was added in liquid N2 atmosphere. It was followed by the addition of 1 g of
barium acetate (Ba(CH3COO)2 ) in 3 mL of isopropanol and 2 mL of distilled water to form
a sol. The sol was then transferred to the polypropylene bottle and kept in the hot air oven at
100 oC for 3 h to form a white colored barium titanate gel. Then it was filtered, washed and
dried at 100 o.C for 3 h. The 1:1 solution of ethanol and HCl was used as the solvent during
washing to extract dodecylamine. It was then followed by the heat treatment at 750 oC for 1h
so as to extract the template completely.
Results and Discussion
Figure 1 gives the x-ray diffraction pattern of BaTiO3 obtained finally after heat treatment at
750 oC for 1h. XRD studies indicated the complete extraction of the template resulting in
the formation of perovskite BaTiO3 with cubic structure (JCPDS no. 75-0212) and the
studies have also revealed the nanocrystalline nature of barium titanate with the average
crystallite size ~20 nm.
Figure 1. XRD pattern of BaTiO3 obtained after subsequent heat treatment at 750 oC for 1 h.
896 T.V. ANURADHA
Figure 2 gives the scanning electron microscopic (SEM) image of barium titanate
obtained here. SEM studies confirmed the porous nature of the product and the particles are
found to be nearly spherical. The formation of agglomerates is evident from the SEM studies
which has the cauli-flower like morphology.
Figure 2. SEM micrograph of BaTiO3 obtained after heat treatment at 750 oC.
Figure 3 gives the bright field transmission electron microscopic (TEM) image of
barium titanate powder with its corresponding selected area electron diffraction (SAED)
pattern and Figure 4 gives its corresponding dark field TEM image. TEM studies indicated
the average particle size to be less than 10 nm.
Figure 3. The bright fild TEM image of BaTiO3 obtained after heat treatment at 750 oC and
(b) its corresponding selected area diffraction pattern.
Figure 4. The dark field image of BaTiO3 produced.
d e f
Template-Assisted Sol-Gel Synthesis of Nanocrystalline BaTiO3 897
The surfactant molecule which is used as the template forms molecular self-assemblies
called micelles with spherical shape in aqueous solutions at a particular concentration called,
first critical micellar concentration (cmc1) and if the concentration exceeds cmc1 and
reaches the second critical micellar concentration (cmc2), the spherical micelle transforms to
the rod-like micelles which then organizes to form liquid-crystalline phases with various
structures as shown in the Figure 5. The spherical micelles can be either normal (with all the
hydrophilic head groups projecting out) or reverse (with all the hydrophilic head groups
projecting in). Formation of mesoporous material involves the normal micellar rods forming
the liquid crystalline mesophase as the template. On the other hand, the reverse micelles
result in the formation of reverse liquid crystalline mesophase which fails to form
mesoporous material through templating, but aids in the formation of nanocrystalline
material by a way of providing the core of the micellar rod containing water as a nano
reactor within which the reaction of the precursors take place. Thus it is believed that the
reverse micellar rods of dodecylamine is formed in these experiments with the controlled
hydrolysis and condensation of the precursors namely Ba(CH3COO)2 and TiCl4 taking place
in its aqueous core which acts as the nano reactor.
Figure 5. Structures of mesostructured phases. The top row shows structures with long-
range order: a) hexagonal phase, b) cubic phase, c) lamellar phase. The bottom row shows
possible disordered structures, as they may occur in some of the mesoporous metal oxides:
d) disordered arrangement of parallel cylindrical pores, e) disordered packing of cylindrical
pores, f) worm-shaped pores.
Nanocrystalline cubic BaTiO3 with the average particle sizes less than ~10 nm is formed by
the condensation and controlled hydrolysis of Ba(CH3COO)2 and TiCl4 in the reverse
micelles of dodecylamine of the reverse hexagonal liquid crystalline phase (mesostructure).
It is evident from the TEM studies that the particle size distribution of sol-gel derived
BaTiO3 is very narrow. Electron microscopic studies indicated that the particle morphology
of BaTiO3 derived by the sol-gel method to be spherical.
The author acknowledges the financial support from CSIR (India) through senior research
fellowship. The author is also thankful to Prof. S. Ranganathan (Department of Materials
Engineering, IISc, Bangalore, India) for his guidance in this research.
898 T.V. ANURADHA
1. Subbarao E C, Prasad V C S and Veerbhadra Rao K, Preparation and characterization
of Materials; Honig J M and Rao C N R, Academic Press, New York, 1981, 217.
2. Setter N and Waser R, Acta Mater., 2000, 48, 151.
3. Lee S K, Park T J, Choi G J, Koo K K and Kim S W, Materials Chem Phys.,
2003, 82, 742.
4. Lemoine C, Gilbert B, Michaux B, Pirard J P and Lecloux A J, J Non-crystalline
Solids, 1994, 175, 1.
5. Zhu X, Zhu J, Zhou S, Liu Z, Ming N and Hesse D, J Crystal Growth., 2005, 283, 553.
6. Guo L, Luo H, Gao J, Guo L and Yang J, Mater Lett., 2006, 60, 3011.
7. Anuradha T V, Ranganathan S, Mimani T and Patil K C, Scripta Materialia 2001, 44,
8. Wang H W, Kuo C H, Liao T H, Lin R J and Cheng S Y, J Mater Res., 2006, 21, 941.
9. Huo R Z, Ferreira P and Vilarinho P M Microporous & Mesoporous Mater.,
2008, 110, 392.
Submit your manuscripts athttp://www.hindawi.com